EVALUATION OF TEST METHODS FOR DETERMINATION OF FORMALDEHYDE EMISSION FROM COMPOSITE WOOD PRODUCTS Mohamed Z.M. SALEM, Martin BÖHM, Jaromír SRBA, Štefan BARCÍK salemmohamed @ fld.czu .cz, bohm @fld.czu.cz
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
EVALUATION OF TEST METHODS FOR DETERMINATION OF
FORMALDEHYDE EMISSION FROM COMPOSITE WOOD PRODUCTS
Mohamed Z.M. SALEM, Martin BÖHM, Jaromír SRBA, Štefan BARCÍK
Department of Wood Processing, Faculty of Forestry and Wood Sciences, Czech University of Life Sciences Prague, Kamycka 1176, 165 21 Prague 6 - Suchdol, Czech Republic
Test chamber with sample
Formaldehyde is mainly used to produce synthetic adhesives by reaction with phenols, urea, and melamine. Urea-formaldehyde resin is a major commercial adhesive, especially within the forest products industry. Composite wood products (CWPs) are usually used for constructing furniture, cabinets, flooring and wall panels for using in commercial and residential structures. However, the toxicity of CWPs bonded with formaldehyde-based resins due to the emission of formaldehyde.
In 1992, the California Air Resources Board (CARB) identified formaldehyde as a toxic air contaminant based primarily on the determination that it was a human carcinogen with no known safe level of exposure. At concentrations above 0.1 ppm in air formaldehyde can irritate the eyes and mucous membranes, resulting in watery eyes. Formaldehyde inhaled at this concentration may cause headaches, a burning sensation in the throat, and difficulty breathing, as well as triggering or aggravating asthma symptoms. In 2004, the International Agency for Research on Cancer (IARC) conducted an evaluation of formaldehyde and concluded that there is sufficient evidence that formaldehyde causes nasopharyngeal cancer in humans.
This work deals with the determination of formaldehyde emission with perforator method (EN 120) and gas analysis method (EN 717-2) from CWPs.
The measured data were evaluated by basic and advanced statistical methods using correlation coefficients between gas analysis and perforator values and the general linear model (GLM) procedure in SAS. One of the main objectives of this work was to evaluate the effectiveness of the lamination on the resultant formaldehyde emissions when applied on PB.
Table 2: Values of formaldehyde content from PB, MDF and PW boards of different types and thicknesses
Approximately 111 different commercial boards shown in Table 1 obtained from a commercial wood manufacturing plant in the Czech Republic were measured for their formaldehyde emissions. All specimens were conditioned to equilibrium at a temperature of 20 °C and 65% relative humidity (RH).
Table 1: Number of specimens used for the gas analysis and perforator tests according to the thickness of the boards.
a: calculated gas analysis value (mg/m2.h).
b: values in parenthesis are the corrected perforator value (mg/100 g) at a moisture content of 6.5 % (EN 312, 2003).
na: data not available.
P2: boards for interior fitments (including furniture) for use in dry conditions (EN 312-2, 2003), PL: laminated particleboard, MDF: general purpose boards for use in dry conditions, MDFL: laminated MDF, PLY: non-structural plywood, PLYs: structural plywood.
Determination of formaldehyde emission in this work was carried out by two approved methods for determining formaldehyde, used at the international level: the gas analysis method and the perforator method
Figure 3: Correlation between EN 717-2 and EN 120 for uncoated particleboards, thickness 18 mm (A)and thickness 12-18 mm (B) and for MDF, thickness 3.2-18 mm (C)
Gas Analysis Method, EN 717-2
This method (Fig. 1) describes determination of the accelerated release of formaldehyde from wood-based panels. A test piece of 400 x 50 mm is placed in a 4-litre cylindrical chamber with controlled temperature (60 °C), RH (≤ 3%), airflow and pressure. Air is continuously passed through the chamber at 1L/min over the test piece, whose edge is sealed with self-adhesive aluminium tape before testing. The gas analysis value (mg/m2.h) depends on the gaseous resistance, density, moisture content, board thickness and airflow rate (Yu and Crump 1999). The emission E1 is ≤ 3.5 mg HCHO/m2.h.
Perforator Method, EN 120
This is a well-established test method widely used in industry; the total operation and analysis time is approximately 3 h (Fig. 2). A sample board of 110 g total, in 25 x 25-mm pieces, is boiled for 2 h using 600 ml toluene under reflux. The formaldehyde is absorbed in the water. After analysis of the extract, the formaldehyde content of the boards is expressed in milligrams per 100 g of dry board and is corrected for moisture content of 6.5% (EN 322). The emission E1 is ≤ 8 mg HCHO/100 g dry coated board and ≤ 12 mg HCHO/100 g dry uncoated board.
Figure 4: The mean effect of particleboard types (A), thicknesses (B) and the interaction between them (C) on the formaldehyde emission measured by EN 717-2
Table 3: The gas analysis values from the different types of particleboard and thicknesses.
Means with the same letter are not significantly different (P<0.05). The small letters on the same column are used to compare between board types of the same thickness, and the capital letters in the same row to compare between thicknesses for the same type of board (Duncan’s multiple-range test).
In this study, the formaldehyde emission from particleboard, MDF and plywood are measured well using either the gas analysis or perforator methods. The correlation between the gas analysis and perforator methods was good. Based on the preliminary results, most of the board types tested has to fulfill the same emission limit of E1. On the other hand, the laminating of particleboard surfaces and the thickness had a great influence on formaldehyde emission. For the production of E1 grade boards, all of the process parameters should be taken into account together.
Figure 1: Gas analysis apparatus (Marutzky, 2008)
This work was supported by the Internal Grant Agency of Czech University of Life Sciences in Prague.
Figure 2 – Perforator apparatus (Marutzky, 2008)
CARB. 1992. Identification of Formaldehyde as a Toxic Air Contaminant. Part A. Exposure Assessment. Technical Support Document, Stationary Source Division, Sacramento, CA. 103 pp.
Duncan, D.B., 1955. Multiple range and multiple F-test. Biometrics 11, 1–42.
EN 120. 1993. Wood–based panels—determination of formaldehyde content—extraction method called perforator method. European Standard, September 1993.
EN 322. 1993. Wood–based panels–determination of moisture content.
EN 717–2. 1994. Wood–based panels—determination of formaldehyde release—Part 2: formaldehyde release by the gas analysis method. European Standard, November 1994.
IARC. 2004. Overall Evaluations on Carcinogenicity to Humans. As Evaluated in IARC Monographs, Vol. 1. International Agency for Research on Cancer, Lyon, France.
Marutzky R. 2008. Global formaldehyde regulations and requirements: Current situation and developments. 6th European Wood-based Panel Symposium, Hanover, October 10th, 2008.
SAS, 1999. What’s New in SAS Software in Version 7 and the Version 8 Developer’s Release. SAS Inst., Inc., Cary, NC, USA.
Yu, C.W.F. and Crump D.R. 1999. Testing for formaldehyde emission from wood–based products–a review. Indoor Built Environment. 8:280–286.